#------------------------------------------------------------------------------
#$Date: 2015-08-05 20:10:24 +0300 (Wed, 05 Aug 2015) $
#$Revision: 152785 $
#$URL: svn://www.crystallography.net/cod/cif/4/51/31/4513198.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4513198
loop_
_publ_author_name
'Watkins-Curry, Pilanda'
'Burnett, Joseph Vade'
'Samanta, Tapas'
'Young, David P.'
'Stadler, Shane'
'Chan, Julia Y.'
_publ_section_title
;
 Strategic Crystal Growth and Physical Properties of Single-Crystalline
 LnCo2Al8(Ln = La--Nd, Sm, Yb)
;
_journal_issue                   7
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              3293
_journal_paper_doi               10.1021/acs.cgd.5b00417
_journal_volume                  15
_journal_year                    2015
_chemical_formula_moiety         'Al8 Co2 Yb'
_chemical_formula_sum            'Al8 Co2 Yb'
_chemical_formula_weight         506.74
_space_group_crystal_system      orthorhombic
_space_group_IT_number           55
_space_group_name_Hall           '-P 2 2ab'
_space_group_name_H-M_alt        'P b a m'
_symmetry_space_group_name_Hall  '-P 2 2ab'
_symmetry_space_group_name_H-M   'P b a m'
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2015-05-27 # Formatted by publCIF
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.4110(10)
_cell_length_b                   14.4260(5)
_cell_length_c                   3.9620(5)
_cell_measurement_temperature    293(2)
_cell_volume                     709.36(11)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    CrystalMaker
_computing_publication_material  'publCIF (Westrip, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS Direct Methods (Sheldrick, 2013)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.978
_diffrn_measurement_device_type  'Bruker Kappa D8 Quest CMOS'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0304
_diffrn_reflns_av_unetI/netI     0.0418
_diffrn_reflns_laue_measured_fraction_full 0.993
_diffrn_reflns_laue_measured_fraction_max 0.978
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            1984
_diffrn_reflns_point_group_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.978
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         31.018
_diffrn_reflns_theta_min         3.267
_diffrn_source                   'I\mS microfocus tube'
_exptl_absorpt_coefficient_mu    18.581
_exptl_absorpt_correction_T_max  0.777
_exptl_absorpt_correction_T_min  0.642
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS(2014)
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    4.745
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Fragment
_exptl_crystal_F_000             912
_exptl_crystal_size_max          0.030
_exptl_crystal_size_mid          0.020
_exptl_crystal_size_min          0.020
_refine_diff_density_max         1.890
_refine_diff_density_min         -1.221
_refine_diff_density_rms         0.287
_refine_ls_extinction_coef       0.0066(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.089
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     70
_refine_ls_number_reflns         1248
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.089
_refine_ls_R_factor_all          0.0397
_refine_ls_R_factor_gt           0.0281
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0249P)²+0.4770P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0606
_refine_ls_wR_factor_ref         0.0649
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1035
_reflns_number_total             1248
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            cg5b00417_si_001.cif
_cod_data_source_block           shelx
_cod_depositor_comments
'Adding full bibliography for 4513193--4513198.cif.'
_cod_database_code               4513198
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.606
_shelx_estimated_absorpt_t_max   0.708
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'x+1/2, -y+1/2, -z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, y, -z'
'-x-1/2, y-1/2, z'
'x-1/2, -y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Yb1 Yb 0.34148(2) 0.31888(2) 0.0000 0.01110(11) Uani 1 2 d S T P
Co1 Co 0.03449(7) 0.40727(5) 0.0000 0.00922(18) Uani 1 2 d S T P
Co2 Co 0.14999(6) 0.09812(5) 0.0000 0.00663(18) Uani 1 2 d S T P
Al1 Al 0.02412(15) 0.13298(12) 0.5000 0.0085(4) Uani 1 2 d S T P
Al2 Al 0.16199(15) 0.37964(13) 0.5000 0.0095(4) Uani 1 2 d S T P
Al3 Al 0.23627(15) 0.17461(12) 0.5000 0.0091(4) Uani 1 2 d S T P
Al4 Al 0.33204(16) 0.49161(13) 0.5000 0.0095(4) Uani 1 2 d S T P
Al5 Al 0.45163(15) 0.18064(12) 0.5000 0.0088(4) Uani 1 2 d S T P
Al6 Al 0.09629(15) 0.25461(11) 0.0000 0.0102(4) Uani 1 2 d S T P
Al7 Al 0.33805(14) 0.04514(14) 0.0000 0.0113(4) Uani 1 2 d S T P
Al8 Al 0.0000 0.5000 0.5000 0.0082(5) Uani 1 4 d S T P
Al9 Al 0.0000 0.0000 0.0000 0.0099(5) Uani 1 4 d S T P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Yb Yb -0.3850 5.5486 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Al1 Yb1 Al1 79.76(5) 3_556 3
Al1 Yb1 Al2 150.62(5) 3_556 1_554
Al1 Yb1 Al2 93.08(4) 3 1_554
Al1 Yb1 Al2 93.08(4) 3_556 .
Al1 Yb1 Al2 150.62(5) 3 .
Al2 Yb1 Al2 79.22(4) 1_554 .
Al1 Yb1 Al5 54.28(4) 3_556 .
Al1 Yb1 Al5 103.23(4) 3 .
Al2 Yb1 Al5 153.84(5) 1_554 .
Al2 Yb1 Al5 95.13(4) . .
Al1 Yb1 Al5 103.23(4) 3_556 1_554
Al1 Yb1 Al5 54.28(4) 3 1_554
Al2 Yb1 Al5 95.13(4) 1_554 1_554
Al2 Yb1 Al5 153.84(5) . 1_554
Al5 Yb1 Al5 78.66(4) . 1_554
Al1 Yb1 Al3 92.83(4) 3_556 .
Al1 Yb1 Al3 148.68(5) 3 .
Al2 Yb1 Al3 106.83(4) 1_554 .
Al2 Yb1 Al3 59.28(5) . .
Al5 Yb1 Al3 50.39(5) . .
Al5 Yb1 Al3 99.09(4) 1_554 .
Al1 Yb1 Al3 148.68(5) 3_556 1_554
Al1 Yb1 Al3 92.83(4) 3 1_554
Al2 Yb1 Al3 59.29(5) 1_554 1_554
Al2 Yb1 Al3 106.83(4) . 1_554
Al5 Yb1 Al3 99.09(4) . 1_554
Al5 Yb1 Al3 50.39(5) 1_554 1_554
Al3 Yb1 Al3 77.76(4) . 1_554
Al1 Yb1 Al6 140.12(2) 3_556 .
Al1 Yb1 Al6 140.12(2) 3 .
Al2 Yb1 Al6 52.87(3) 1_554 .
Al2 Yb1 Al6 52.87(3) . .
Al5 Yb1 Al6 103.44(4) . .
Al5 Yb1 Al6 103.44(4) 1_554 .
Al3 Yb1 Al6 53.99(4) . .
Al3 Yb1 Al6 53.99(4) 1_554 .
Al1 Yb1 Al4 104.47(4) 3_556 1_554
Al1 Yb1 Al4 56.80(4) 3 1_554
Al2 Yb1 Al4 49.95(5) 1_554 1_554
Al2 Yb1 Al4 98.60(4) . 1_554
Al5 Yb1 Al4 155.41(5) . 1_554
Al5 Yb1 Al4 96.95(3) 1_554 1_554
Al3 Yb1 Al4 153.00(5) . 1_554
Al3 Yb1 Al4 96.33(3) 1_554 1_554
Al6 Yb1 Al4 101.12(4) . 1_554
Al1 Yb1 Al4 56.80(4) 3_556 .
Al1 Yb1 Al4 104.47(4) 3 .
Al2 Yb1 Al4 98.60(4) 1_554 .
Al2 Yb1 Al4 49.95(5) . .
Al5 Yb1 Al4 96.95(3) . .
Al5 Yb1 Al4 155.41(5) 1_554 .
Al3 Yb1 Al4 96.33(3) . .
Al3 Yb1 Al4 153.00(5) 1_554 .
Al6 Yb1 Al4 101.12(4) . .
Al4 Yb1 Al4 76.91(4) 1_554 .
Al1 Yb1 Al9 51.62(3) 3_556 3
Al1 Yb1 Al9 51.62(3) 3 3
Al2 Yb1 Al9 101.88(4) 1_554 3
Al2 Yb1 Al9 101.88(4) . 3
Al5 Yb1 Al9 104.28(3) . 3
Al5 Yb1 Al9 104.28(3) 1_554 3
Al3 Yb1 Al9 140.86(2) . 3
Al3 Yb1 Al9 140.86(2) 1_554 3
Al6 Yb1 Al9 143.92(3) . 3
Al4 Yb1 Al9 52.93(3) 1_554 3
Al4 Yb1 Al9 52.93(3) . 3
Al6 Co1 Al8 125.322(16) . .
Al6 Co1 Al8 125.322(16) . 1_554
Al8 Co1 Al8 109.33(3) . 1_554
Al6 Co1 Al7 124.93(7) . 3_455
Al8 Co1 Al7 71.40(3) . 3_455
Al8 Co1 Al7 71.40(3) 1_554 3_455
Al6 Co1 Al7 122.30(7) . 7_665
Al8 Co1 Al7 71.25(3) . 7_665
Al8 Co1 Al7 71.25(3) 1_554 7_665
Al7 Co1 Al7 112.77(5) 3_455 7_665
Al6 Co1 Al2 69.54(5) . .
Al8 Co1 Al2 64.19(4) . .
Al8 Co1 Al2 145.48(5) 1_554 .
Al7 Co1 Al2 129.46(3) 3_455 .
Al7 Co1 Al2 74.80(5) 7_665 .
Al6 Co1 Al2 69.54(5) . 1_554
Al8 Co1 Al2 145.48(5) . 1_554
Al8 Co1 Al2 64.19(4) 1_554 1_554
Al7 Co1 Al2 129.46(3) 3_455 1_554
Al7 Co1 Al2 74.80(5) 7_665 1_554
Al2 Co1 Al2 101.04(7) . 1_554
Al6 Co1 Al5 70.44(5) . 3_455
Al8 Co1 Al5 146.21(5) . 3_455
Al8 Co1 Al5 64.66(3) 1_554 3_455
Al7 Co1 Al5 75.42(5) 3_455 3_455
Al7 Co1 Al5 129.49(3) 7_665 3_455
Al2 Co1 Al5 139.98(6) . 3_455
Al2 Co1 Al5 64.82(5) 1_554 3_455
Al6 Co1 Al5 70.44(5) . 3_456
Al8 Co1 Al5 64.66(3) . 3_456
Al8 Co1 Al5 146.21(5) 1_554 3_456
Al7 Co1 Al5 75.42(5) 3_455 3_456
Al7 Co1 Al5 129.49(3) 7_665 3_456
Al2 Co1 Al5 64.82(5) . 3_456
Al2 Co1 Al5 139.98(6) 1_554 3_456
Al5 Co1 Al5 101.01(7) 3_455 3_456
Al6 Co1 Co1 178.54(7) . 5_565
Al8 Co1 Co1 54.664(15) . 5_565
Al8 Co1 Co1 54.664(15) 1_554 5_565
Al7 Co1 Co1 56.53(5) 3_455 5_565
Al7 Co1 Co1 56.24(5) 7_665 5_565
Al2 Co1 Co1 109.62(5) . 5_565
Al2 Co1 Co1 109.62(5) 1_554 5_565
Al5 Co1 Co1 110.40(5) 3_455 5_565
Al5 Co1 Co1 110.40(5) 3_456 5_565
Al9 Co2 Al6 110.80(5) . .
Al9 Co2 Al7 124.62(6) . .
Al6 Co2 Al7 124.58(7) . .
Al9 Co2 Al3 127.32(4) . 1_554
Al6 Co2 Al3 72.48(5) . 1_554
Al7 Co2 Al3 74.40(5) . 1_554
Al9 Co2 Al3 127.32(4) . .
Al6 Co2 Al3 72.48(5) . .
Al7 Co2 Al3 74.40(5) . .
Al3 Co2 Al3 104.36(7) 1_554 .
Al9 Co2 Al4 72.60(5) . 7_654
Al6 Co2 Al4 127.63(4) . 7_654
Al7 Co2 Al4 74.09(6) . 7_654
Al3 Co2 Al4 66.99(5) 1_554 7_654
Al3 Co2 Al4 148.49(7) . 7_654
Al9 Co2 Al4 72.60(5) . 7_655
Al6 Co2 Al4 127.63(4) . 7_655
Al7 Co2 Al4 74.09(6) . 7_655
Al3 Co2 Al4 148.49(7) 1_554 7_655
Al3 Co2 Al4 66.99(5) . 7_655
Al4 Co2 Al4 103.82(7) 7_654 7_655
Al9 Co2 Al1 68.59(4) . 1_554
Al6 Co2 Al1 68.94(5) . 1_554
Al7 Co2 Al1 129.64(4) . 1_554
Al3 Co2 Al1 64.21(5) 1_554 1_554
Al3 Co2 Al1 141.41(6) . 1_554
Al4 Co2 Al1 64.34(5) 7_654 1_554
Al4 Co2 Al1 141.19(6) 7_655 1_554
Al9 Co2 Al1 68.59(4) . .
Al6 Co2 Al1 68.94(5) . .
Al7 Co2 Al1 129.64(4) . .
Al3 Co2 Al1 141.41(6) 1_554 .
Al3 Co2 Al1 64.21(5) . .
Al4 Co2 Al1 141.19(6) 7_654 .
Al4 Co2 Al1 64.34(5) 7_655 .
Al1 Co2 Al1 100.72(7) 1_554 .
Co2 Al1 Co2 100.72(7) 1_556 .
Co2 Al1 Al3 56.73(4) 1_556 .
Co2 Al1 Al3 56.73(4) . .
Co2 Al1 Al4 56.84(4) 1_556 7_655
Co2 Al1 Al4 56.83(4) . 7_655
Al3 Al1 Al4 61.65(7) . 7_655
Co2 Al1 Al9 118.71(7) 1_556 .
Co2 Al1 Al9 51.71(2) . .
Al3 Al1 Al9 105.01(6) . .
Al4 Al1 Al9 63.30(4) 7_655 .
Co2 Al1 Al9 51.71(2) 1_556 1_556
Co2 Al1 Al9 118.71(7) . 1_556
Al3 Al1 Al9 105.01(6) . 1_556
Al4 Al1 Al9 63.30(4) 7_655 1_556
Al9 Al1 Al9 91.15(5) . 1_556
Co2 Al1 Al6 51.83(4) 1_556 1_556
Co2 Al1 Al6 118.30(8) . 1_556
Al3 Al1 Al6 63.11(6) . 1_556
Al4 Al1 Al6 105.15(7) 7_655 1_556
Al9 Al1 Al6 167.25(9) . 1_556
Al9 Al1 Al6 87.85(3) 1_556 1_556
Co2 Al1 Al6 118.30(8) 1_556 .
Co2 Al1 Al6 51.83(4) . .
Al3 Al1 Al6 63.11(6) . .
Al4 Al1 Al6 105.15(7) 7_655 .
Al9 Al1 Al6 87.85(3) . .
Al9 Al1 Al6 167.25(9) 1_556 .
Al6 Al1 Al6 90.32(7) 1_556 .
Co2 Al1 Al5 112.21(5) 1_556 3_456
Co2 Al1 Al5 112.21(5) . 3_456
Al3 Al1 Al5 95.65(8) . 3_456
Al4 Al1 Al5 157.30(9) 7_655 3_456
Al9 Al1 Al5 128.43(4) . 3_456
Al9 Al1 Al5 128.43(4) 1_556 3_456
Al6 Al1 Al5 60.40(5) 1_556 3_456
Al6 Al1 Al5 60.40(5) . 3_456
Co2 Al1 Al4 111.55(5) 1_556 3_456
Co2 Al1 Al4 111.55(5) . 3_456
Al3 Al1 Al4 155.84(9) . 3_456
Al4 Al1 Al4 94.18(7) 7_655 3_456
Al9 Al1 Al4 59.83(4) . 3_456
Al9 Al1 Al4 59.83(4) 1_556 3_456
Al6 Al1 Al4 129.35(5) 1_556 3_456
Al6 Al1 Al4 129.35(5) . 3_456
Al5 Al1 Al4 108.51(8) 3_456 3_456
Co2 Al1 Yb1 169.51(6) 1_556 3_455
Co2 Al1 Yb1 89.755(19) . 3_455
Al3 Al1 Yb1 131.71(5) . 3_455
Al4 Al1 Yb1 130.72(5) 7_655 3_455
Al9 Al1 Yb1 67.56(3) . 3_455
Al9 Al1 Yb1 122.29(6) 1_556 3_455
Al6 Al1 Yb1 123.28(7) 1_556 3_455
Al6 Al1 Yb1 68.86(4) . 3_455
Al5 Al1 Yb1 63.51(4) 3_456 3_455
Al4 Al1 Yb1 63.22(4) 3_456 3_455
Co2 Al1 Yb1 89.755(19) 1_556 3_456
Co2 Al1 Yb1 169.51(6) . 3_456
Al3 Al1 Yb1 131.71(5) . 3_456
Al4 Al1 Yb1 130.72(5) 7_655 3_456
Al9 Al1 Yb1 122.29(6) . 3_456
Al9 Al1 Yb1 67.56(3) 1_556 3_456
Al6 Al1 Yb1 68.86(4) 1_556 3_456
Al6 Al1 Yb1 123.28(7) . 3_456
Al5 Al1 Yb1 63.51(4) 3_456 3_456
Al4 Al1 Yb1 63.22(4) 3_456 3_456
Yb1 Al1 Yb1 79.76(5) 3_455 3_456
Co1 Al2 Co1 101.04(7) . 1_556
Co1 Al2 Al8 55.38(4) . .
Co1 Al2 Al8 55.38(4) 1_556 .
Co1 Al2 Al4 113.28(6) . .
Co1 Al2 Al4 113.28(6) 1_556 .
Al8 Al2 Al4 101.76(8) . .
Co1 Al2 Al5 57.60(4) . 3_456
Co1 Al2 Al5 57.60(4) 1_556 3_456
Al8 Al2 Al5 59.24(5) . 3_456
Al4 Al2 Al5 160.99(10) . 3_456
Co1 Al2 Al6 51.28(4) . .
Co1 Al2 Al6 117.81(7) 1_556 .
Al8 Al2 Al6 101.57(6) . .
Al4 Al2 Al6 128.51(5) . .
Al5 Al2 Al6 61.33(5) 3_456 .
Co1 Al2 Al6 117.81(7) . 1_556
Co1 Al2 Al6 51.28(4) 1_556 1_556
Al8 Al2 Al6 101.57(6) . 1_556
Al4 Al2 Al6 128.51(5) . 1_556
Al5 Al2 Al6 61.33(5) 3_456 1_556
Al6 Al2 Al6 90.05(7) . 1_556
Co1 Al2 Yb1 89.64(2) . .
Co1 Al2 Yb1 167.94(6) 1_556 .
Al8 Al2 Yb1 136.63(3) . .
Al4 Al2 Yb1 66.55(5) . .
Al5 Al2 Yb1 126.23(5) 3_456 .
Al6 Al2 Yb1 64.92(4) . .
Al6 Al2 Yb1 118.56(7) 1_556 .
Co1 Al2 Yb1 167.93(6) . 1_556
Co1 Al2 Yb1 89.64(2) 1_556 1_556
Al8 Al2 Yb1 136.63(4) . 1_556
Al4 Al2 Yb1 66.55(5) . 1_556
Al5 Al2 Yb1 126.23(5) 3_456 1_556
Al6 Al2 Yb1 118.56(7) . 1_556
Al6 Al2 Yb1 64.92(4) 1_556 1_556
Yb1 Al2 Yb1 79.22(4) . 1_556
Co2 Al3 Co2 104.36(7) 1_556 .
Co2 Al3 Al5 116.17(5) 1_556 .
Co2 Al3 Al5 116.17(5) . .
Co2 Al3 Al1 59.06(4) 1_556 .
Co2 Al3 Al1 59.06(4) . .
Al5 Al3 Al1 169.01(9) . .
Co2 Al3 Al4 56.67(4) 1_556 7_655
Co2 Al3 Al4 56.67(4) . 7_655
Al5 Al3 Al4 109.67(8) . 7_655
Al1 Al3 Al4 59.35(7) . 7_655
Co2 Al3 Al6 117.56(8) 1_556 .
Co2 Al3 Al6 51.29(4) . .
Al5 Al3 Al6 126.20(5) . .
Al1 Al3 Al6 60.03(5) . .
Al4 Al3 Al6 101.38(6) 7_655 .
Co2 Al3 Al6 51.29(4) 1_556 1_556
Co2 Al3 Al6 117.56(8) . 1_556
Al5 Al3 Al6 126.20(5) . 1_556
Al1 Al3 Al6 60.02(5) . 1_556
Al4 Al3 Al6 101.38(6) 7_655 1_556
Al6 Al3 Al6 87.05(7) . 1_556
Co2 Al3 Yb1 88.34(2) 1_556 1_556
Co2 Al3 Yb1 164.30(6) . 1_556
Al5 Al3 Yb1 64.22(4) . 1_556
Al1 Al3 Yb1 123.37(6) . 1_556
Al4 Al3 Yb1 138.97(3) 7_655 1_556
Al6 Al3 Yb1 114.68(6) . 1_556
Al6 Al3 Yb1 63.45(4) 1_556 1_556
Co2 Al3 Yb1 164.30(6) 1_556 .
Co2 Al3 Yb1 88.34(2) . .
Al5 Al3 Yb1 64.22(4) . .
Al1 Al3 Yb1 123.37(6) . .
Al4 Al3 Yb1 138.97(3) 7_655 .
Al6 Al3 Yb1 63.45(4) . .
Al6 Al3 Yb1 114.68(6) 1_556 .
Yb1 Al3 Yb1 77.76(4) 1_556 .
Co2 Al4 Co2 103.82(7) 7_666 7_665
Co2 Al4 Al2 116.19(6) 7_666 .
Co2 Al4 Al2 116.19(6) 7_665 .
Co2 Al4 Al1 58.82(4) 7_666 7_665
Co2 Al4 Al1 58.82(4) 7_665 7_665
Al2 Al4 Al1 168.63(10) . 7_665
Co2 Al4 Al3 56.35(4) 7_666 7_665
Co2 Al4 Al3 56.35(4) 7_665 7_665
Al2 Al4 Al3 109.62(9) . 7_665
Al1 Al4 Al3 59.00(7) 7_665 7_665
Co2 Al4 Al9 50.84(3) 7_666 3_556
Co2 Al4 Al9 116.86(7) 7_665 3_556
Al2 Al4 Al9 126.92(5) . 3_556
Al1 Al4 Al9 59.42(4) 7_665 3_556
Al3 Al4 Al9 100.45(6) 7_665 3_556
Co2 Al4 Al9 116.86(7) 7_666 3
Co2 Al4 Al9 50.84(3) 7_665 3
Al2 Al4 Al9 126.92(5) . 3
Al1 Al4 Al9 59.42(4) 7_665 3
Al3 Al4 Al9 100.45(6) 7_665 3
Al9 Al4 Al9 86.99(5) 3_556 3
Co2 Al4 Al1 107.26(6) 7_666 3_556
Co2 Al4 Al1 107.26(6) 7_665 3_556
Al2 Al4 Al1 105.56(8) . 3_556
Al1 Al4 Al1 85.81(7) 7_665 3_556
Al3 Al4 Al1 144.82(9) 7_665 3_556
Al9 Al4 Al1 56.43(4) 3_556 3_556
Al9 Al4 Al1 56.43(4) 3 3_556
Co2 Al4 Al7 115.18(8) 7_666 7_665
Co2 Al4 Al7 52.03(4) 7_665 7_665
Al2 Al4 Al7 66.24(6) . 7_665
Al1 Al4 Al7 105.67(7) 7_665 7_665
Al3 Al4 Al7 62.56(6) 7_665 7_665
Al9 Al4 Al7 162.65(8) 3_556 7_665
Al9 Al4 Al7 92.54(3) 3 7_665
Al1 Al4 Al7 135.87(4) 3_556 7_665
Co2 Al4 Al7 52.03(4) 7_666 7_666
Co2 Al4 Al7 115.18(8) 7_665 7_666
Al2 Al4 Al7 66.24(6) . 7_666
Al1 Al4 Al7 105.67(7) 7_665 7_666
Al3 Al4 Al7 62.56(6) 7_665 7_666
Al9 Al4 Al7 92.54(3) 3_556 7_666
Al9 Al4 Al7 162.65(8) 3 7_666
Al1 Al4 Al7 135.87(4) 3_556 7_666
Al7 Al4 Al7 82.78(7) 7_665 7_666
Co2 Al4 Yb1 164.53(6) 7_666 .
Co2 Al4 Yb1 89.13(2) 7_665 .
Al2 Al4 Yb1 63.50(5) . .
Al1 Al4 Yb1 124.36(6) 7_665 .
Al3 Al4 Yb1 139.11(3) 7_665 .
Al9 Al4 Yb1 115.74(6) 3_556 .
Al9 Al4 Yb1 65.05(3) 3 .
Al1 Al4 Yb1 59.98(4) 3_556 .
Al7 Al4 Yb1 79.42(4) 7_665 .
Al7 Al4 Yb1 129.70(7) 7_666 .
Co2 Al4 Yb1 89.13(2) 7_666 1_556
Co2 Al4 Yb1 164.53(6) 7_665 1_556
Al2 Al4 Yb1 63.50(5) . 1_556
Al1 Al4 Yb1 124.36(6) 7_665 1_556
Al3 Al4 Yb1 139.11(3) 7_665 1_556
Al9 Al4 Yb1 65.05(3) 3_556 1_556
Al9 Al4 Yb1 115.74(6) 3 1_556
Al1 Al4 Yb1 59.98(4) 3_556 1_556
Al7 Al4 Yb1 129.70(7) 7_665 1_556
Al7 Al4 Yb1 79.42(4) 7_666 1_556
Yb1 Al4 Yb1 76.91(4) . 1_556
Co1 Al5 Co1 101.01(7) 3 3_556
Co1 Al5 Al3 112.60(5) 3 .
Co1 Al5 Al3 112.60(5) 3_556 .
Co1 Al5 Al8 55.15(4) 3 3_556
Co1 Al5 Al8 55.15(4) 3_556 3_556
Al3 Al5 Al8 101.11(7) . 3_556
Co1 Al5 Al2 57.58(4) 3 3_556
Co1 Al5 Al2 57.58(4) 3_556 3_556
Al3 Al5 Al2 159.71(9) . 3_556
Al8 Al5 Al2 58.61(5) 3_556 3_556
Co1 Al5 Al6 116.67(8) 3 3_556
Co1 Al5 Al6 50.89(4) 3_556 3_556
Al3 Al5 Al6 130.12(5) . 3_556
Al8 Al5 Al6 100.32(6) 3_556 3_556
Al2 Al5 Al6 60.18(5) 3_556 3_556
Co1 Al5 Al6 50.89(4) 3 3
Co1 Al5 Al6 116.67(8) 3_556 3
Al3 Al5 Al6 130.12(5) . 3
Al8 Al5 Al6 100.32(6) 3_556 3
Al2 Al5 Al6 60.18(5) 3_556 3
Al6 Al5 Al6 88.78(7) 3_556 3
Co1 Al5 Al1 109.96(5) 3 3_556
Co1 Al5 Al1 109.96(6) 3_556 3_556
Al3 Al5 Al1 110.36(8) . 3_556
Al8 Al5 Al1 148.53(8) 3_556 3_556
Al2 Al5 Al1 89.92(8) 3_556 3_556
Al6 Al5 Al1 59.07(5) 3_556 3_556
Al6 Al5 Al1 59.07(5) 3 3_556
Co1 Al5 Yb1 168.37(5) 3 1_556
Co1 Al5 Yb1 90.076(19) 3_556 1_556
Al3 Al5 Yb1 65.39(4) . 1_556
Al8 Al5 Yb1 136.05(3) 3_556 1_556
Al2 Al5 Yb1 128.07(5) 3_556 1_556
Al6 Al5 Yb1 67.88(4) 3_556 1_556
Al6 Al5 Yb1 120.68(7) 3 1_556
Al1 Al5 Yb1 62.21(4) 3_556 1_556
Co1 Al5 Yb1 90.076(19) 3 .
Co1 Al5 Yb1 168.36(5) 3_556 .
Al3 Al5 Yb1 65.39(4) . .
Al8 Al5 Yb1 136.05(3) 3_556 .
Al2 Al5 Yb1 128.07(5) 3_556 .
Al6 Al5 Yb1 120.68(6) 3_556 .
Al6 Al5 Yb1 67.88(4) 3 .
Al1 Al5 Yb1 62.21(4) 3_556 .
Yb1 Al5 Yb1 78.66(4) 1_556 .
Co1 Al6 Co2 177.25(9) . .
Co1 Al6 Al1 119.19(6) . .
Co2 Al6 Al1 59.23(5) . .
Co1 Al6 Al1 119.19(6) . 1_554
Co2 Al6 Al1 59.23(5) . 1_554
Al1 Al6 Al1 90.32(7) . 1_554
Co1 Al6 Al2 59.17(5) . 1_554
Co2 Al6 Al2 122.36(6) . 1_554
Al1 Al6 Al2 178.08(9) . 1_554
Al1 Al6 Al2 89.79(4) 1_554 1_554
Co1 Al6 Al2 59.17(5) . .
Co2 Al6 Al2 122.36(6) . .
Al1 Al6 Al2 89.79(4) . .
Al1 Al6 Al2 178.08(9) 1_554 .
Al2 Al6 Al2 90.05(7) 1_554 .
Co1 Al6 Al5 58.67(5) . 3_455
Co2 Al6 Al5 119.72(6) . 3_455
Al1 Al6 Al5 119.99(8) . 3_455
Al1 Al6 Al5 60.52(5) 1_554 3_455
Al2 Al6 Al5 58.49(5) 1_554 3_455
Al2 Al6 Al5 117.84(7) . 3_455
Co1 Al6 Al5 58.67(5) . 3_456
Co2 Al6 Al5 119.72(6) . 3_456
Al1 Al6 Al5 60.52(5) . 3_456
Al1 Al6 Al5 119.99(8) 1_554 3_456
Al2 Al6 Al5 117.84(7) 1_554 3_456
Al2 Al6 Al5 58.49(5) . 3_456
Al5 Al6 Al5 88.78(7) 3_455 3_456
Co1 Al6 Al3 125.28(5) . .
Co2 Al6 Al3 56.23(4) . .
Al1 Al6 Al3 56.86(5) . .
Al1 Al6 Al3 115.46(7) 1_554 .
Al2 Al6 Al3 124.73(8) 1_554 .
Al2 Al6 Al3 66.13(5) . .
Al5 Al6 Al3 175.52(8) 3_455 .
Al5 Al6 Al3 91.92(4) 3_456 .
Co1 Al6 Al3 125.28(5) . 1_554
Co2 Al6 Al3 56.23(4) . 1_554
Al1 Al6 Al3 115.46(7) . 1_554
Al1 Al6 Al3 56.86(5) 1_554 1_554
Al2 Al6 Al3 66.13(5) 1_554 1_554
Al2 Al6 Al3 124.73(8) . 1_554
Al5 Al6 Al3 91.92(4) 3_455 1_554
Al5 Al6 Al3 175.52(8) 3_456 1_554
Al3 Al6 Al3 87.05(7) . 1_554
Co1 Al6 Yb1 92.26(6) . .
Co2 Al6 Yb1 90.50(6) . .
Al1 Al6 Yb1 119.32(6) . .
Al1 Al6 Yb1 119.32(6) 1_554 .
Al2 Al6 Yb1 62.21(5) 1_554 .
Al2 Al6 Yb1 62.21(5) . .
Al5 Al6 Yb1 120.69(5) 3_455 .
Al5 Al6 Yb1 120.68(5) 3_456 .
Al3 Al6 Yb1 62.56(5) . .
Al3 Al6 Yb1 62.56(5) 1_554 .
Co1 Al6 Yb1 89.33(6) . 3_455
Co2 Al6 Yb1 87.92(5) . 3_455
Al1 Al6 Yb1 59.76(5) . 3_455
Al1 Al6 Yb1 59.76(5) 1_554 3_455
Al2 Al6 Yb1 118.74(5) 1_554 3_455
Al2 Al6 Yb1 118.74(5) . 3_455
Al5 Al6 Yb1 60.25(5) 3_455 3_455
Al5 Al6 Yb1 60.25(5) 3_456 3_455
Al3 Al6 Yb1 116.43(5) . 3_455
Al3 Al6 Yb1 116.43(5) 1_554 3_455
Yb1 Al6 Yb1 178.41(6) . 3_455
Co2 Al7 Co1 146.14(9) . 3
Co2 Al7 Co1 146.63(9) . 7_655
Co1 Al7 Co1 67.23(5) 3 7_655
Co2 Al7 Al8 136.84(2) . 3_556
Co1 Al7 Al8 52.62(3) 3 3_556
Co1 Al7 Al8 52.56(3) 7_655 3_556
Co2 Al7 Al8 136.84(2) . 3
Co1 Al7 Al8 52.62(3) 3 3
Co1 Al7 Al8 52.56(3) 7_655 3
Al8 Al7 Al8 86.31(5) 3_556 3
Co2 Al7 Al4 53.89(5) . 7_654
Co1 Al7 Al4 138.42(3) 3 7_654
Co1 Al7 Al4 103.70(6) 7_655 7_654
Al8 Al7 Al4 152.03(8) 3_556 7_654
Al8 Al7 Al4 88.78(3) 3 7_654
Co2 Al7 Al4 53.89(5) . 7_655
Co1 Al7 Al4 138.42(3) 3 7_655
Co1 Al7 Al4 103.70(6) 7_655 7_655
Al8 Al7 Al4 88.78(3) 3_556 7_655
Al8 Al7 Al4 152.03(8) 3 7_655
Al4 Al7 Al4 82.78(7) 7_654 7_655
Co1 Al8 Co1 109.33(3) 5_566 5_565
Co1 Al8 Co1 70.67(3) 5_566 1_556
Co1 Al8 Co1 180.0 5_565 1_556
Co1 Al8 Co1 180.00(3) 5_566 .
Co1 Al8 Co1 70.67(3) 5_565 .
Co1 Al8 Co1 109.33(3) 1_556 .
Co1 Al8 Al2 119.57(2) 5_566 .
Co1 Al8 Al2 119.57(2) 5_565 .
Co1 Al8 Al2 60.43(2) 1_556 .
Co1 Al8 Al2 60.43(2) . .
Co1 Al8 Al2 60.43(2) 5_566 5_566
Co1 Al8 Al2 60.43(2) 5_565 5_566
Co1 Al8 Al2 119.57(2) 1_556 5_566
Co1 Al8 Al2 119.57(2) . 5_566
Al2 Al8 Al2 180.0 . 5_566
Co1 Al8 Al5 60.18(2) 5_566 7_665
Co1 Al8 Al5 60.18(2) 5_565 7_665
Co1 Al8 Al5 119.82(2) 1_556 7_665
Co1 Al8 Al5 119.82(2) . 7_665
Al2 Al8 Al5 117.84(6) . 7_665
Al2 Al8 Al5 62.16(6) 5_566 7_665
Co1 Al8 Al5 119.82(2) 5_566 3_456
Co1 Al8 Al5 119.82(2) 5_565 3_456
Co1 Al8 Al5 60.18(2) 1_556 3_456
Co1 Al8 Al5 60.18(2) . 3_456
Al2 Al8 Al5 62.16(6) . 3_456
Al2 Al8 Al5 117.84(6) 5_566 3_456
Al5 Al8 Al5 180.0 7_665 3_456
Co1 Al8 Al7 55.98(4) 5_566 7_666
Co1 Al8 Al7 123.81(4) 5_565 7_666
Co1 Al8 Al7 56.19(4) 1_556 7_666
Co1 Al8 Al7 124.02(4) . 7_666
Al2 Al8 Al7 67.78(4) . 7_666
Al2 Al8 Al7 112.23(4) 5_566 7_666
Al5 Al8 Al7 67.98(5) 7_665 7_666
Al5 Al8 Al7 112.02(5) 3_456 7_666
Co1 Al8 Al7 124.02(4) 5_566 3_455
Co1 Al8 Al7 56.19(4) 5_565 3_455
Co1 Al8 Al7 123.81(4) 1_556 3_455
Co1 Al8 Al7 55.98(4) . 3_455
Al2 Al8 Al7 112.22(4) . 3_455
Al2 Al8 Al7 67.77(4) 5_566 3_455
Al5 Al8 Al7 112.02(5) 7_665 3_455
Al5 Al8 Al7 67.98(5) 3_456 3_455
Al7 Al8 Al7 180.0 7_666 3_455
Co1 Al8 Al7 56.19(4) 5_566 3_456
Co1 Al8 Al7 124.02(4) 5_565 3_456
Co1 Al8 Al7 55.98(4) 1_556 3_456
Co1 Al8 Al7 123.81(4) . 3_456
Al2 Al8 Al7 112.22(4) . 3_456
Al2 Al8 Al7 67.77(4) 5_566 3_456
Al5 Al8 Al7 112.02(5) 7_665 3_456
Al5 Al8 Al7 67.98(5) 3_456 3_456
Al7 Al8 Al7 93.69(5) 7_666 3_456
Al7 Al8 Al7 86.31(5) 3_455 3_456
Co1 Al8 Al7 123.81(4) 5_566 7_665
Co1 Al8 Al7 55.98(4) 5_565 7_665
Co1 Al8 Al7 124.02(4) 1_556 7_665
Co1 Al8 Al7 56.19(4) . 7_665
Al2 Al8 Al7 67.78(4) . 7_665
Al2 Al8 Al7 112.23(4) 5_566 7_665
Al5 Al8 Al7 67.98(5) 7_665 7_665
Al5 Al8 Al7 112.02(5) 3_456 7_665
Al7 Al8 Al7 86.31(5) 7_666 7_665
Al7 Al8 Al7 93.69(5) 3_455 7_665
Al7 Al8 Al7 180.0 3_456 7_665
Co2 Al9 Co2 180.0 . 5
Co2 Al9 Al1 120.30(4) . 5
Co2 Al9 Al1 59.70(4) 5 5
Co2 Al9 Al1 120.30(4) . 5_556
Co2 Al9 Al1 59.70(4) 5 5_556
Al1 Al9 Al1 91.15(5) 5 5_556
Co2 Al9 Al1 59.70(4) . 1_554
Co2 Al9 Al1 120.30(4) 5 1_554
Al1 Al9 Al1 88.85(5) 5 1_554
Al1 Al9 Al1 180.00(9) 5_556 1_554
Co2 Al9 Al1 59.70(4) . .
Co2 Al9 Al1 120.30(4) 5 .
Al1 Al9 Al1 180.0 5 .
Al1 Al9 Al1 88.85(5) 5_556 .
Al1 Al9 Al1 91.15(5) 1_554 .
Co2 Al9 Al4 56.56(4) . 7_655
Co2 Al9 Al4 123.44(4) 5 7_655
Al1 Al9 Al4 122.73(5) 5 7_655
Al1 Al9 Al4 63.74(5) 5_556 7_655
Al1 Al9 Al4 116.26(5) 1_554 7_655
Al1 Al9 Al4 57.28(5) . 7_655
Co2 Al9 Al4 123.44(4) . 3_455
Co2 Al9 Al4 56.56(4) 5 3_455
Al1 Al9 Al4 57.27(5) 5 3_455
Al1 Al9 Al4 116.26(5) 5_556 3_455
Al1 Al9 Al4 63.74(5) 1_554 3_455
Al1 Al9 Al4 122.72(5) . 3_455
Al4 Al9 Al4 180.00(5) 7_655 3_455
Co2 Al9 Al4 56.56(4) . 7_654
Co2 Al9 Al4 123.44(4) 5 7_654
Al1 Al9 Al4 63.74(5) 5 7_654
Al1 Al9 Al4 122.73(5) 5_556 7_654
Al1 Al9 Al4 57.27(5) 1_554 7_654
Al1 Al9 Al4 116.26(5) . 7_654
Al4 Al9 Al4 86.99(5) 7_655 7_654
Al4 Al9 Al4 93.01(5) 3_455 7_654
Co2 Al9 Al4 123.44(4) . 3_456
Co2 Al9 Al4 56.56(4) 5 3_456
Al1 Al9 Al4 116.26(5) 5 3_456
Al1 Al9 Al4 57.27(5) 5_556 3_456
Al1 Al9 Al4 122.73(5) 1_554 3_456
Al1 Al9 Al4 63.74(5) . 3_456
Al4 Al9 Al4 93.01(5) 7_655 3_456
Al4 Al9 Al4 86.99(5) 3_455 3_456
Al4 Al9 Al4 180.00(9) 7_654 3_456
Co2 Al9 Yb1 89.73(2) . 3_455
Co2 Al9 Yb1 90.27(2) 5 3_455
Al1 Al9 Yb1 119.18(4) 5 3_455
Al1 Al9 Yb1 119.18(4) 5_556 3_455
Al1 Al9 Yb1 60.82(4) 1_554 3_455
Al1 Al9 Yb1 60.82(4) . 3_455
Al4 Al9 Yb1 117.99(3) 7_655 3_455
Al4 Al9 Yb1 62.01(3) 3_455 3_455
Al4 Al9 Yb1 117.99(3) 7_654 3_455
Al4 Al9 Yb1 62.01(3) 3_456 3_455
Co2 Al9 Yb1 90.27(2) . 7_655
Co2 Al9 Yb1 89.73(2) 5 7_655
Al1 Al9 Yb1 60.82(4) 5 7_655
Al1 Al9 Yb1 60.82(4) 5_556 7_655
Al1 Al9 Yb1 119.18(4) 1_554 7_655
Al1 Al9 Yb1 119.18(4) . 7_655
Al4 Al9 Yb1 62.01(3) 7_655 7_655
Al4 Al9 Yb1 117.99(3) 3_455 7_655
Al4 Al9 Yb1 62.01(3) 7_654 7_655
Al4 Al9 Yb1 117.99(3) 3_456 7_655
Yb1 Al9 Yb1 180.0 3_455 7_655
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Yb1 Al1 3.0895(15) 3_556
Yb1 Al1 3.0895(15) 3
Yb1 Al2 3.1072(14) 1_554
Yb1 Al2 3.1073(14) .
Yb1 Al5 3.1257(14) .
Yb1 Al5 3.1257(14) 1_554
Yb1 Al3 3.1561(14) .
Yb1 Al3 3.1561(14) 1_554
Yb1 Al6 3.1812(19) .
Yb1 Al4 3.1854(15) 1_554
Yb1 Al4 3.1854(15) .
Yb1 Al9 3.2707(3) 3
Co1 Al6 2.3320(18) .
Co1 Al8 2.4284(5) .
Co1 Al8 2.4284(5) 1_554
Co1 Al7 2.533(2) 3_455
Co1 Al7 2.541(2) 7_665
Co1 Al2 2.5666(13) .
Co1 Al2 2.5666(13) 1_554
Co1 Al5 2.5672(12) 3_455
Co1 Al5 2.5672(12) 3_456
Co1 Co1 2.8089(16) 5_565
Co2 Al9 2.3386(8) .
Co2 Al6 2.3539(18) .
Co2 Al7 2.456(2) .
Co2 Al3 2.5077(12) 1_554
Co2 Al3 2.5077(12) .
Co2 Al4 2.5170(13) 7_654
Co2 Al4 2.5170(13) 7_655
Co2 Al1 2.5725(13) 1_554
Co2 Al1 2.5725(13) .
Al1 Co2 2.5725(13) 1_556
Al1 Al3 2.701(3) .
Al1 Al4 2.710(3) 7_655
Al1 Al9 2.7738(12) .
Al1 Al9 2.7738(12) 1_556
Al1 Al6 2.7939(17) 1_556
Al1 Al6 2.7939(17) .
Al1 Al5 2.835(2) 3_456
Al1 Al4 2.985(3) 3_456
Al1 Yb1 3.0895(15) 3_455
Al1 Yb1 3.0895(15) 3_456
Al2 Co1 2.5666(13) 1_556
Al2 Al8 2.6564(19) .
Al2 Al4 2.658(3) .
Al2 Al5 2.752(3) 3_456
Al2 Al6 2.8004(18) .
Al2 Al6 2.8004(18) 1_556
Al2 Yb1 3.1073(14) 1_556
Al3 Co2 2.5077(12) 1_556
Al3 Al5 2.674(3) .
Al3 Al4 2.773(3) 7_655
Al3 Al6 2.8766(19) .
Al3 Al6 2.8766(19) 1_556
Al3 Yb1 3.1560(14) 1_556
Al4 Co2 2.5170(13) 7_666
Al4 Co2 2.5170(13) 7_665
Al4 Al1 2.710(3) 7_665
Al4 Al3 2.773(3) 7_665
Al4 Al9 2.8783(14) 3_556
Al4 Al9 2.8783(14) 3
Al4 Al1 2.985(3) 3_556
Al4 Al7 2.996(2) 7_665
Al4 Al7 2.996(2) 7_666
Al4 Yb1 3.1854(15) 1_556
Al5 Co1 2.5672(12) 3
Al5 Co1 2.5672(12) 3_556
Al5 Al8 2.6742(17) 3_556
Al5 Al2 2.752(3) 3_556
Al5 Al6 2.8319(19) 3_556
Al5 Al6 2.8319(19) 3
Al5 Al1 2.835(2) 3_556
Al5 Yb1 3.1257(14) 1_556
Al6 Al1 2.7939(17) 1_554
Al6 Al2 2.8004(18) 1_554
Al6 Al5 2.8319(19) 3_455
Al6 Al5 2.8319(19) 3_456
Al6 Al3 2.8766(19) 1_554
Al6 Yb1 3.3354(19) 3_455
Al7 Co1 2.533(2) 3
Al7 Co1 2.541(2) 7_655
Al7 Al8 2.8962(13) 3_556
Al7 Al8 2.8962(13) 3
Al7 Al4 2.996(2) 7_654
Al7 Al4 2.996(2) 7_655
Al8 Co1 2.4283(5) 5_566
Al8 Co1 2.4283(5) 5_565
Al8 Co1 2.4283(5) 1_556
Al8 Al2 2.6565(19) 5_566
Al8 Al5 2.6742(17) 7_665
Al8 Al5 2.6742(17) 3_456
Al8 Al7 2.8962(13) 7_666
Al8 Al7 2.8962(13) 3_455
Al8 Al7 2.8962(13) 3_456
Al8 Al7 2.8962(13) 7_665
Al9 Co2 2.3387(8) 5
Al9 Al1 2.7738(12) 5
Al9 Al1 2.7738(12) 5_556
Al9 Al1 2.7738(12) 1_554
Al9 Al4 2.8783(14) 7_655
Al9 Al4 2.8783(14) 3_455
Al9 Al4 2.8783(14) 7_654
Al9 Al4 2.8783(14) 3_456
Al9 Yb1 3.2707(3) 3_455
Al9 Yb1 3.2707(3) 7_655
